advertisement

APPLIED PHYSICS LETTERS 97, 062504 共2010兲 Rate-dependence of the switching field distribution in nanoscale granular magnetic materials O. Hovorka,1,a兲 R. F. L. Evans,2 R. W. Chantrell,2 and A. Berger1 1 CIC nanoGUNE Consolider, Donostia-San Sebastián, 20018, Spain Department of Physics, The University of York, Heslington, York YO10 5DD, United Kingdom 2 共Received 2 July 2010; accepted 20 July 2010; published online 11 August 2010兲 The external field sweep-rate dependence of the intrinsic switching field distribution in perpendicular recording media is investigated. We derive a scaling relationship for switching field distributions at different sweep-rates, which we then validate by means of large-scale kinetic Monte Carlo simulations based on interacting Stoner–Wohlfarth particles. After demonstrating the possible occurrence of large differences between switching field distributions at slow time scales of conventional magnetometry and very fast processes relevant in magnetic recording, we propose a technique for extrapolating between these very different sweep-rates. © 2010 American Institute of Physics. 关doi:10.1063/1.3477956兴 Magnetic information storage relies on recording and preserving information in nanoscale magnetic grains that are generally coupled by magnetostatic and exchange interactions.1 The presence of these interactions considerably complicates magnetization processes as well as the extraction of local materials properties from macroscopic measurements. An important example of this problem is the identification of intrinsic switching field distributions D共HS兲 from macroscopic hysteresis loops in highly anisotropic granular magnetic materials, which are being used for magnetic recording. D共HS兲 is defined as the distribution of switching thresholds of individual particles in the interaction-free case and it is a crucial materials property for magnetic recording as it directly determines the local precision of bit transitions.2 D共HS兲 is related to the anisotropy field distribution D共HK兲 of grains, from which it mostly differs due to thermal activation, which introduces additional relaxational time scales and leads to a dependence of the particle switching field on the external magnetic field sweep rate R.3 It also leads to a dependence from the volume distribution D共V兲 of the grains because the activation barrier for the thermal relaxation phenomena is volume dependent. A general relationship between D共HS兲 measured at different sweep rates and between D共HS兲 and D共HK兲 is not known and will be a subject of the present study. A recent experimental study on perpendicular recording materials 共PMRs兲 共Refs. 4 and 5兲 demonstrated a 50% difference between the relative widths of D共HS兲 measured at time scales of a typical laboratory magnetometry 共R ⬃ 102 Oe/ s兲 and time scales more closely related to magnetic recording 共R ⬃ 108 Oe/ s兲. In these experiments the relative width of D共HS兲 was quantified by the ratio of the standard deviation to the coercive field, S / HC, as is conventional. Similar experimental observations in terms of the squareness Sⴱ of the hysteresis loops have also been reported very recently.6 The problem of identifying the rate dependence of D共HS兲 partly arises from the fact that extracting D共HS兲 from hysteresis loops in interacting particle assemblies is typically Author to whom correspondence should be addressed. Tel.: ⫹34 943 574 000. FAX: ⫹34 943 574 001. Electronic mail: [email protected] a兲 0003-6951/2010/97共6兲/062504/3/$30.00 a very difficult problem and techniques developed for this purpose7–15 rely on various degrees of approximations. Importantly, they essentially ignore thermal relaxation effects and it is unclear how accurately the methods relate to the fast subnanosecond time scale relevant for write processes in hard disk drives. In the present work, we investigate this issue by using a kinetic Monte Carlo model of PMR materials. We find that the recently developed version of the ⌬H共M , ⌬M兲-methodology13,14 allows accurate extraction of S of D共HS兲 from the computed hysteresis loops even in the presence of exchange and dipolar interactions. Having demonstrated the accurate determination of S, we then study theoretically the rate-dependence of S / HC showing that slow time scale measurements can overestimate the relative width K / HK of D共HK兲 by as much as 300%. We also derive a scaling relationship, which relates S / HC and K / HK for different R. Following Ref. 16, the well established kinetic Monte Carlo modeling framework assumes a planar assembly of N Stoner–Wohlfarth 共SW兲 particles i of volume V distributed on a hexagonal lattice of spacing a. The magnetization of every particle normalized by the saturation value MS is described by a dimensionless unit vector free to rotate. The uniaxial anisotropy axes of particles are oriented perpendicular to the film plane collinear with the external field of strength Ha. It is assumed that the anisotropy constants Ki and correspondingly the anisotropy fields HK,i = 2Ki / MS 共CGS units兲 vary randomly from particle to particle according to the lognormal probability distribution having mean 2 典 具HK,i典, median HK, and standard deviation K = 共具HK,i 2 1/2 − 具HK典 兲 . For reasons of transparency of the present work we will ignore distributions of anisotropy axis orientations D共␣兲 and volumes D共V兲 of the particles.17 The nearest neighbor exchange interactions are quantified by an exchange field constant HEX, which is the total exchange field on a particle in the saturation state. The longrange magnetostatic coupling between the grains is approximated by dipolar interactions. Thermal switching involves the evaluation of particle-dependent energy barriers ⌬E separating positive and negative magnetization states of the particles using the effective field concept. We assume thermal transitions to be governed by the Arrhenius–Néel relaxation law w⫾ = f0 exp共−⌬E⫾ / kBT兲, where w+ and w− are the tran- 97, 062504-1 © 2010 American Institute of Physics Author complimentary copy. Redistribution subject to AIP license or copyright, see http://apl.aip.org/apl/copyright.jsp 062504-2 Appl. Phys. Lett. 97, 062504 共2010兲 Hovorka et al. summarize the derivation, as it will be used later for our generalization toward switching field distributions. Considering the physical picture leading here to Eq. 共1兲, the switching threshold HS,i of a single SW particle with anisotropy HK,i and the thermal stability ratio i corresponds 2 典 to its coercivity; HS,i = HC,i. Then the S = 共具HC,i 2 1/2 − 具HC,i典 兲 . Due to the thermal relaxation HS,i ⬍ HK,i but they coincide in the nonrelaxational case for tm → 0 共or equivalently R → ⬁兲. The dependence of HC,i on R can be evaluated by integrating Eq. 共1兲 over the hysteresis process generated by a magnetic field decreasing at the rate R and starting from saturation. This yields the following:19 1/2 HC,i = HK,i兵1 − 关−1 i ln共tif0兲兴 其 FIG. 1. 共Color online兲 Dependence of the coercive field HC on the external field sweep rate R for different thermal stability factors for the noninteracting case 共䊊兲 and the case with dipolar interactions and exchange HEX = 10 kOe共⌬兲. Lines represent the least-square fits of Eq. 共3兲. Inset: Dependence of ⴱ obtained from fitting Eq. 共3兲 for 0 ⱕ HEX ⱕ 10 kOe. sition rates for escaping from the positive and negative states, respectively, f0 is the attempt frequency factor, kB is the Boltzmann constant, and T is the temperature. The particle-dependent characteristic relaxation time depends on w⫾ and equals to = 1 / 共w+ + w−兲. The actual probabilities for switching between the particle states are given by the following: P共tm兲 = P0 exp共− tm/兲 + w+关1 − exp共− tm/兲兴, 共1兲 which results as a solution of the corresponding singleparticle master equation.16 In Eq. 共1兲, P0 is the probability of finding a particle in the negative state initially at Ha and P共tm兲 is the probability of preserving that state after the time step tm. For an external field changing in constant steps ⌬Ha the field sweep-rate is defined as R = ⌬Ha / tm. In simulations, we compute hysteresis loops, including recoil curves which are required below for the identification of D共HS兲 using the ⌬H共M , ⌬M兲-method.13,14 We assume a system of N = 160⫻ 160 particles with lattice spacing a = 8 nm and grain heights L = 5.5, 8, and 12 nm. Setting MS = 400 emu/ cc, T = 300 K, and 具HK,i典 = 40 kOe 共HK = 38 kOe兲, this gives thermal stability ratios  = KV/ kBT = 54, 77, and 116. We set K / HK = 0.2. This choice of parameter sets is guided by the boundary of what is relevant for typical recording media design or might be so in the future,2 where thermal relaxation effects will be especially important. However, our results are general within the range of validity of the assumed Arrhenius–Néel relaxation picture, i.e., they are not reliant on any specific parameter set. We first analyze the sweep-rate dependence of the dynamic coercive field HC obtained from the computed hysteresis loops. Figure 1 shows HC共R兲 for different HEX and . Exchange interactions cause a squaring up of the hysteresis loops and an increase in HC, which becomes more pronounced for reduced . The dependence of HC on the measurement time scale is typically quantified by Sharrock’s equation in case of a relaxational experiment18 or by similar equations relevant for swept-field experiments,19 which is the case here. We briefly 共2兲 with ti = 共2iR兲−1HK,i共1 − HC,i / HK,i兲−1, being the effective time. Integrating this equation over the anisotropy distribution D共HK兲 in the noninteracting particle case gives a macroscopic version of Eq. 共2兲 applicable in the noninteracting case: HC = HK兵1 − 关−1 ln共tf0兲兴1/2其, with t = 共2R兲−1HK共1 − HC / HK兲−1 and HC and HK representing, respectively, the median of HC,i and HK,i.20 This equation is normally fitted also to interacting particle assemblies in which case HK and  are interaction-dependent fit parameters and will be distinguished using the standard notation as H0 and ⴱ, respectively. Thus the macroscopic analogy of Eq. 共2兲 is as follows: HC = H0兵1 − 关ⴱ−1 ln共tf0兲兴1/2其 ⴱ 共3兲 and t = 共2 R兲 H0共1 − HC / H0兲 , defines the effective time as previously.21 According to Fig. 1, Eq. 共3兲 fits the HC versus R data very well for all interactions despite the fact that it was derived using the noninteracting particle picture. The inset shows that the fit parameter ⴱ increases with HEX, which relates to the increase in the effective activation volume due to the stabilizing exchange interaction. Nonetheless we note that the resulting fit values correspond to the preset values of  rather well. In addition, H0 is found to vary only slightly with HEX. We now address the issue of R-dependence of the standard deviation S of D共HS兲. Figure 2共a兲 shows S obtained from hysteresis loops using the ⌬H共M , ⌬M兲-method.13,14 Although other available methods can be used for extracting S as well, we found here that the ⌬H共M , ⌬M兲-method accurately represents the intrinsic S for all R and in the entire range of exchange interactions considered. For instance, this can be seen from the figure where practically all data points for HEX = 10 kOe fall on top of the noninteracting case line corresponding to a given . We note that in the noninteracting case S was confirmed to agree with the differentiated major loop which directly corresponds to D共HS兲. In the noninteracting case the dependence S versus R can also be calculated analytically. Squaring both sides of Eq. 共2兲, expressing the mean and the second moment over the distribution D共HK兲, and using the same assumptions as above20 gives the following: −1 −1 S = K兵1 − S关−1 ln共tf0兲兴1/2其 with S = 冉 冊 −1/2 2 1/2 典 具HK,i典 − 具HK,i 具HK,i典 2 . 具HK,i典 − 具HK,i典2 共4a兲 共4b兲 The factor S is dependent only on the properties of the underlying anisotropy distribution D共HK兲 and is independent of Author complimentary copy. Redistribution subject to AIP license or copyright, see http://apl.aip.org/apl/copyright.jsp 062504-3 Appl. Phys. Lett. 97, 062504 共2010兲 Hovorka et al. and 2共b兲 show that after rescaling the axis all data collapse well onto a single line, further validating the approach in the presence of interactions. In summary, numerical calculations based on the kinetic Monte Carlo SW-model show that the laboratory time scale measured S / HC can substantially overestimate the intrinsic K / HK; by as much as 300% within the R range considered. Techniques to obtain S, such as the ⌬H共M , ⌬M兲-method used in this work, have only been demonstrated at slow rates R. We propose a powerful and precise experimental procedure for extrapolating to the S / HC at recording frequencies, which is the truly relevant characteristic related to magnetic recording. The procedure is based on a combination of ratedependent magnetometry, specifically HC versus R measurements and a single R measurement of hysteresis loop data needed for applying the ⌬H共M , ⌬M兲-method. Work at nanoGUNE acknowledges the EROTEK Program, Project No. IE06-172 and the Spanish Ministry of Science and Education Project No. CSD2006-53. O.H. acknowledges the Marie Curie International Reintegration Grant Project No. 224924. 1 S. N. Piramanayagam and K. Srinivasan, J. Magn. Magn. Mater. 321, 485 共2009兲. H. J. Richter and S. D. Harkness, MRS Bull. 31, 384 共2006兲. 3 D. Weller and A. Moser, IEEE Trans. Magn. 35, 4423 共1999兲. 4 T. Shimatsu, T. Kondo, K. Mitsuzuka, S. Watanabe, H. Aoi, H. Muraoka, and Y. Nakamura, IEEE Trans. Magn. 43, 2091 共2007兲. 5 T. Shimatsu, T. Kondo, K. Mitsuzuka, S. Watanabe, H. Aoi, H. Muraoka, and Y. Nakamura, J. Appl. Phys. 99, 08F905 共2006兲. 6 K. Srinivasan, B. Ramamurthy Acharya, and G. Bertero, J. Appl. Phys. 107, 113912 共2010兲. 7 M. Winklhofer and G. T. Zimanyi, J. Appl. Phys. 99, 08E710 共2006兲. 8 X. Wu and R. J. M. van de Veerdonk, IEEE Trans. Magn. 44, 336 共2008兲. 9 R. J. M. van de Veerdonk, X. Wu, and D. Weller, IEEE Trans. Magn. 39, 590 共2003兲. 10 A. Berger, B. Lengsfield, and Y. Ikeda, J. Appl. Phys. 99, 08E705 共2006兲. 11 O. Hellwig, A. Berger, T. Thomson, E. Dobisz, Z. Z. Bandic, H. Yang, D. S. Kercher, and E. E. Fullerton, Appl. Phys. Lett. 90, 162516 共2007兲. 12 Y. Liu, K. A. Dahmen, and A. Berger, Appl. Phys. Lett. 92, 222503 共2008兲. 13 O. Hovorka, Y. Liu, K. A. Dahmen, and A. Berger, J. Magn. Magn. Mater. 322, 459 共2010兲. 14 O. Hovorka, Y. Liu, K. A. Dahmen, and A. Berger, Appl. Phys. Lett. 95, 192504 共2009兲. 15 C. Papusoi, Jr., Phys. Lett. A 265, 391 共2000兲. 16 R. W. Chantrell, N. Walmsley, J. Gore, and M. Maylin, Phys. Rev. B 63, 024410 共2000兲. 17 These distributions will generally result in an additional broadening of the magnetization transition and a decorrelation between the ratios S / HC and K / HK. A quantification, in how far D共␣兲 and D共V兲 modify the result and the overall scaling relations found here, will be a subject of future studies. 18 M. P. Sharrock, J. Appl. Phys. 76, 6413 共1994兲. 19 R. W. Chantrell, G. N. Coverdale, and K. O’Grady, J. Phys. D: Appl. Phys. 21, 1469 共1988兲. 20 Derivation assumes 共1兲 具关ln共tif0兲兴1/2典 ⬃ 关ln共具ti典f0兲兴1/2 = 关ln共tf0兲兴1/2, with the notation 具ti典 = t, and that ti is only weakly correlated with HK,i. This is reasonable because i is proportional to HK,i and because of the anticorrelation nature the ratio HC,i / HK,i, which results in a sharply peaked probability distribution for ti centered around the mean t. 共2兲 That the coercive field characterizes switching of the most typical particles in the medium, which is the case for magnetic recording materials, to allow neglecting higher order covariance terms. We also note, that equivalent equation holds for mean values 具HC,i典, 具i典, and 具HK,i典 as long as the differences 具HC,i典-HC and 具HK,i典-HK are not too large and follow similar trends as a function of R. 21 Note that t does not appear in the case of the Sharrock equation, which applies to different experimental procedures based on measuring the remanent coercivity.3,18 Note also, that it is easier to fit the inverted Eq. 共3兲, i.e., after expressing R as a function of HC. 2 FIG. 2. 共Color online兲 共a兲 Dependence of the switching field distribution width S on the external field sweep rate R for different thermal stability factors for the non-interacting case 共䊊兲 and the case with dipolar interactions and exchange HEX = 10 kOe共⌬兲. Lines represent plots of Eq. 共4兲 using H0 and ⴱ obtained from fitting Eq. 共3兲 to HC共R兲. Inset: A collapse of all the fitted curves onto a universal function y = 1 – 2−1关ln共1 / x兲兴1/2 after rescaling the axes. ␣ = 2ⴱ共1 − HC / H0兲 / H0. 共b兲 The same as 共a兲 but for the ratio S / HC given by Eq. 共5兲. Inset: the universal function has now the following form: y = 兵1 – 2−1关ln共1 / x兲兴1/2其 / 兵1 − 关ln共1 / x兲兴1/2其. R or any quantities related to thermal relaxation. S can be calculated exactly for a lognormal distribution which gives S ⬃ 1 / 2 for our numerical examples 共S = 1 / 2 for a symmetric distribution兲. Although Eq. 共4兲 has been derived assuming the noninteracting particle picture, Fig. 2共a兲 shows that it also reproduces well the data for the interacting case if the interactiondependent parameters ⴱ and H0 obtained from fitting Eq. 共3兲 are used. Similarly, using Eqs. 共3兲 and 共4兲 a general relationship between S / HC and K / HK can be expressed in the following form: 1 − 关ⴱ−1 ln共tf0兲兴1/2 K S = ⫻ , H0 HC 1 – 2−1关ⴱ−1 ln共tf0兲兴1/2 共5兲 with t = 共2ⴱR兲−1H0共1 − HC / H0兲−1 as before and after using S = 1 / 2 for the lognormal distribution. Equation 共5兲 allows determining the intrinsic K / H0 based on the ⴱ and H0 obtained from fitting Eq. 共3兲 and S obtained by the ⌬H共M , ⌬M兲-method. Figure 2共b兲 shows excellent agreement between the computed data and Eq. 共5兲. Insets in Figs. 2共a兲 Author complimentary copy. Redistribution subject to AIP license or copyright, see http://apl.aip.org/apl/copyright.jsp